SHEAR BEHAVIOR OF REINFORCED CONCRETE BEAMS

WITH

A SMALL AMOUNT OF WEB REINFORCEMENT

Songkram Piyamahant

A dissertation submitted to

Kochi University of Technology

in partial fulfillment of the requirements for

The Degree of Master of Engineering

Supervisor

Professor Hiroshi Shima

Department of Infrastructure System Engineering

Kochi University of Technology

Kochi, Japan

January 2002

Abstract

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

i

ABSTRACT

In 1995, Hyogoken-nambu Earthquake destroyed many of Shinkansen viaduct

structures that were a very large column section, approximately 900 mm., and a small

amount of web reinforcement. With respect to this evidence, the shear strength formula

was clarified in size effect but it still does not clarify the superposition method when a

small amount of web reinforcement is extremely employed. Following that, the aim of

this research is based on shear behavior and superposition method V

cr

+V

s

by intending

on a minimal amount of web reinforcement. Accordingly, 4 reinforced concrete

specimens with web reinforcement ratio equal 0.035%, 0.05%, 0.065%, and 0.08%

were conducted under monotonic loading. Moreover, two measuring systems for

aggregate interlocking and shear resisted by web reinforcement were designed to use in

investigating shear resistance mechanism. Consequently, the experiment shows that

shear carrying capacity of 3 smallest amount of web reinforcement is the same and the

superposition method is safe to predict the shear carrying capacity of reinforced

concrete beam with a small amount of web reinforcement as shear span ratio 3.0.

Similarly, other design codes also show the same degree of safety as the superposition

method is employed. Not only that, but also the result of aggregate interlocking shows

the same amount of stress transfer across the crack since the larger crack width

corresponding to larger sliding of crack surface possesses the same stress transfer as that

of smaller crack width and sliding.

Acknowledgements

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

ii

ACKNOWLEDGEMENTS

I would like to express my deepest gratitude to my advisor Professor Hiroshi Shima for

his kind encouragement and valuable advice throughout the course of this study. I

express my profound gratitude to Professor Hajime Okamura for his guidance especially

on the current problem of reinforced concrete and his encouragement during the course

of this study. My grateful appreciation is extended to Professor Masahiro Ouchi for his

suggestions. It has been an honor and a privilege to work with them for their

outstanding examples of scientific dedication in their field.

Grateful acknowledgements are also extended to Professor Mikio Kadota for their

interest and serving as members of examination committee.

Sincere words of gratitude are expressed to Mr. Masaru Ueno for his useful advice and

support in experimental work.

I also would like to thank Mr.Supakit Swatekititham and Mr.Thammanoon

Dengpongpan, and all of graduate students for their help, support and patience towards

many of my problems during the course of the experimental work.

Table of Contents

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

iii

TABLE OF CONTENTS

Abstract i

Acknowledgements ii

Table of contents iii

1. GENERAL INTRODUCTION

1.1 General and Problem Definition 1-3

1.2 Literature Review 4-6

1.3 Research Objective 7

1.4 Research Strategy and Content 7-8

1.5 References 9-10

2. EXPERIMENTAL DETAILS

2.1 Specimens Detail 11-13

2.2 Measuring Systems 13-20

2.3 Experimental Procedures 20

2.4 References 21

3. EXPERIMENTAL RESULTS AND INVESTIGATION

3.1 Strength and Determination Comparison 22

3.2 Discussion on Experimental Results 22-30

3.3 Conclusion 30

3.4 References 31

4. MECHANICAL IN SHEAR RESISNTANCE

4.1 Mechanism of Stress Transfer 32-36

4.2 Mechanism of Web Reinforcement 37

4.3 Conclusion 38

4.4 References 39

5. CONCLUSION 40

6. RECOMMENDATIONS OF FURTHER STUDY 41

APPENDIX A Crack Mapping

APPENDIX B Crack Deformation at Shear Cracking of Each Beam

CHAPTER 1

GENERAL INTRODUCTION

General and Problem Definition

Literature Review

Research Objective

Research Strategy and Content

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 1

GENERAL INTRODUCTION

1.1 GENERAL AND PROBLEM DEFINITION

Amount of stirrup has a direct relation on the behavior of reinforced concrete

members of general structure, since the structures are possible to fail in brittle manner

without any warning sign if the shear stress rides over the shear carrying capacity.

Great example of shear failure is the collapse of super-structures during Great-

Hanshin Earthquake, in 1995. With respect to that evident, many of viaducts

structures constructed as a rigid-framed [1] were destructed as shown in Figure 1-1.

According to the mentioned structure, the amount of stirrup was lightly used.

Therefore, the following question has been asked by many researchers for such a long

time that did the estimation of shear strength of those was miscalculated?

Figure.1_1: Collapsed Structure.

One of possible and discovered reason is the size effect of the structure members,

which was introduced by Okamura [2]. With respect to this reason, the formula

derived from the specimen in experiments, which are very tiny compare to the real

structure, did not include some important factor. It can be illustrated that strength of

small specimens in experiments are affected in crack propagation by the reinforcing

bar, so called bond effect, which increased the fracture energy of concrete.

Nevertheless, in actual, the effect of bond from the reinforcement is very tiny since

the members cross-section is so large that crack propagation is not able to confine by

bond effect of reinforcement. It used to clarify and accept this problem, size effect, by

many researchers and the consideration in its was added as size effect term in the

shear strength design formula.

Another possible problem but it does not clarify yet is the shear carrying capacity’s

design concept since the concept is used as the strength of concrete at either failure or

shear crack load and sum up with shear resistance of web reinforcement. Why the

shear strength design concept seems to be not enough, it is possible that a small

amount of web reinforcement cannot maintain the shear strength resist by concrete to

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 2

be the same up to yielding point of stirrup itself. The remaining and possible reason is

going to study and describe in this research thesis.

1.1.1 Current Use of Stirrup

As mentioned, the important factors drives shear failure in super-structure during

Kobe’s earthquake was explored. One factor originally based on the past design code

since it used to overestimate in size-effect. A related consideration is because Japan

Society of Civil Engineering’s design guide at the constructing period used allowable

stress design concept, and it had required a suddenly increasing of stirrup if the

allowable shear strength of concrete did not enough as Figure 1-2. Consequently,

escaping from suddenly increasing of stirrup, enlarge section of member to increase

the allowable shear stress in concrete was commonly done. In summary, large section

and small amount of stirrup are the consequence of designing that finally destructed

by the earthquake.

Figure.1_2: Evolution of Stirrup in Design Code.

To solve the problem, the amount of stirrup was later renewed and published by JSCE

again in late year. Accordingly, the minimum requirement of stirrup was strictly

assigned to 0.2% for the beneficial in seismic performances. Although, the designed

structures follows the requirement have resulted in too much material used recently.

In the last, it is possibly that the good shear strength prediction method for whole

range of stirrup can reduce that of necessary cost.

1.1.2 Generality and Applicable of Superimposition Method

By considering simplicity, the several design guides stated that the shear carrying

capacity can be determined by adding the contribution of shear carrying capacity of

concrete with that of stirrup. Whatever the shear strength of concrete are proposed in

many design guide, they are assumed that shear carrying capacity of concrete remains

the same up to the yielding of stirrups if the minimum requirement of stirrup is

provided. As it was claimed about small amount of web reinforcement, this is possible

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 3

that the shear carrying capacity of concrete can not remain constant until the yielding

of stirrup, and again this will result in ineffective calculation by V

c

+ V

s

as shown in

Figure1-3.

Figure.1_3: Assumption on Load Carrying Capacity by Varying Stirrup.

Shear Strength Prediction in Varying Amount of

Web Reinforcement ratio

0.6

1

1.4

0.00

0.05

0.10

0.15

0.20

0.25

Web reinforcement ratio

(%)

V

experiment

/V

calculation

Vexp/(Vc+Vs)

Vexp/(Vcrk+Vs)

Vcrk/Vniwa

Figure.1_4: Prediction of shear strength by superposition method by varying web ratio.

To clarify and preliminary study, Figure.1_4 is the plot along the web reinforcement

ratio, x-axis, by comparing the shear strength calculated by Niwa’s equation [3], and

the assumption of 45 degrees crack to the member axis with the experimental. The

data used in the plotted graph are the large beams that tested in monotonic 3 and 4

point bending with depth higher than 500 mm., and contain quite small until very

small amount of stirrup [4]-[9]. Beyond the web reinforcement ratio about 0.08%, it is

clearly observed that the superposition method is safe enough to determine the shear

carrying capacity. Although it is seemingly that the estimation by superposition

method is not good enough. In summarize, the assumption and real experimental data,

even they were rarely discovered in research publications, are given us reasonable

idea that the shear strength of reinforced concrete beam with a small amount of web

reinforcement can not simplicity determine by superposition method.

V

s

v

w,min = 0.2%

V

c

V

apply

V

c

+V

s

(prediction)

(Test results)

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 4

1.2 LITERATURE REVIEW

1.2.1 Mechanical and Determining of Shear resistance

Generally, as in Figure.1_5, the shear resisting mechanism of reinforced concrete can

be qualitatively classified upon their behaviors as; 1.) Shear stress of concrete in

compression zone; 2.) Aggregate interlocking along the crack plane; 3.) Dowel action

of longitudinal reinforcement; 4.) Stirrup. Although, it is difficult to quantify the

quantitative model in estimating shear resistance of concrete part item by item.

Figure.1_5: General Mechanical of Shear Resistance.

By considering that difficulty, many researchers [3,10] proposed the model to

calculate the shear crack load of reinforced concrete without web reinforcement at

shear cracking level by relying on the collected experimental results. Therefore, the

shear strength of reinforced concrete beams with stirrup can be finally determined by

adding that of concrete and stirrup based on 45-degree truss analogy. Those shear

crack load can be determined by the following equation;

Okamura’s Equation:

dpccr

adfV 14.175.020.0

31

'

1-1

1

wp

p

1

41

d

d

Niwa’s Equation:

addfpV

cwcr

4.175.02.0

41

31

'

1-2

Where, f

c

’

: compressive strength

a : shear span length

d : effective depth

p

w

: tensile reinforcement ratio

In somewhat advance concept, both concrete and stirrup are recognized to possess

some interaction between them. Those were known as beneficial to the beam action

[11] by effectively increasing in; 1.) The dowel action, because of the support offered

by stirrups to longitudinal bars; 2.) The strength of concrete tooth, due to an inclined

compression field associated with truss mechanism; 3.) The aggregate interlock

strength. With respect to this, it shown that stirrup effectiveness can be defined by

‘stirrup effectiveness function’ [12] as 1-3 and 1-4, which is also function of moment

induced in beam action, M

b

, as shown.

pkI

b

1-3

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 5

ucbb

MMI 1-4

Where, k, p : constant

I

b

: beam action index

M

b

: moment contributed by beam action

M

uc

: ultimate moment

Conceptually, it can be said that the amount of stirrup has the direct relations to the

shear resistance by increasing the effectiveness of beam action. Accordingly, in this

terminology, shear strength contributed by concrete was remained constant, no effect

of stirrup effectiveness, but changed in term of shear resisted by stirrup for

simplifying. Shear strength of beams with web reinforcement can be determined by

equation 1-5

scu

VVV 1-5

According to the advance concerning, the shear carrying capacity of reinforced

concrete beam in concrete part after cracking should not be regard to be the same as

just crack [13] but it should be changed. However, in that experiment, the amount of

stirrup used as much more larger than the minimum requirement. Nevertheless, at

least, the behaviors of it after cracking like either load resistance or crack opening and

crack sliding, which control the load-deformation of itself, it mainly depends on the

amount of stirrup.

In summary, the shear carrying capacity of reinforced concrete beam with web

reinforcement does not simply sum up that of concrete and stirrup together as V

c

+V

s

,

but it has to concern with the interaction between them, which actually depend on

amount of web reinforcement.

1.2.2 Provision of Minimum Stirrup in Several Design Codes

As aforementioned, the shear carrying capacity of reinforced concrete beam with web

reinforcement can be simply calculated by V

c

+V

s

, which the shear force resisted by

stirrup has to provide almost minimum not less than the code specified below since it

is assumed that shear force resisted by concrete will remain the same. The following

requirement is the minimum requirement of stirrup according to many designing

codes.

JSCE 1986 [14]

Seismic design code :

s

= 0.20%

ACI 318-83 [15]

Normal strength concrete (Fc’ < 69 Mpa)

y

w

v

f

sb

A

33.0

:

s

= 0.08 – 0.13%

ACI 318-89 [16]

High strength concrete (Fc’ > 69 Mpa)

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 6

y

wc

v

f

sbf

A

33.0

35

'

:

s

> 0.08

CSA 84 (Canada standard association) [17]

y

w

v

f

sb

A

35.0

:

s

= 0.08 – 0.13%

CSA 94 [18]

y

w

cv

f

sb

fA

'

06.0

AASHTO (LRFD Bridge design specification 1994) [19]

y

w

cv

f

sb

fA

'

083.0

Krauthammer [20]

y

w

v

f

sb

A

448.0

:

s

= 0.1 – 0.16%

All of current codes same as that of ACI, CSA, and AASHTO, already provided the

minimum requirement of stirrup for high strength concrete since the higher strength of

concrete affect in more brittle behavior and less shear transfer. Nevertheless, the shear

carrying capacity has some possibilities to be less than the calculation even the

minimum stirrup was provided, this is because the shear carrying capacity of concrete

are not exactly predicted, which clearly observes in the case of ACI code due to either

size effect or lightly reinforcement [4].

1.2.3 Shear Strength of Lightly Web Reinforcment Used

In case that the shear strength has to examine corresponding to the less amount of

stirrup than minimum requirement that guidance is not provided in any design code,

Angelakos, Bentz, and Collins [4] suggested to estimate by using the interpolation

method. This method is to interpolate by tracing the straight line between shear

strength without web reinforcement and full AASHTO minimum amount of stirrups

using as shown in Figure.1_6.

Figure.1_6: Proposed method to determine shear strength of beams with less than

AASHTO specified minimum stirrups

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 7

1.3 RESEARCH OBJECTIVE

Nowadays, in Japan, the existing reinforced concrete structures used the stirrup at

least equal to the minimum requirement specified in JSCE design guide; although, no

theoretical insists that the amount of stirrup equals to 0.2% is appropriate, and how to

determine shear carrying capacity as a small amount of web reinforcement used.

Up to this point of concerning, first objective of this study is to clarify the applicable

of the superposition method that used in predicting shear carrying capacity of

reinforced concrete beam with a small amount of web reinforcement at the shear span

ratio 3.0. Parallel to the first objective, second objective is to make clear that what

mechanisms take place when small amount of stirrup used. In summary, the great

understanding of reinforced concrete member with a small amount of stirrup can be

presented and hit it into shatter.

1.4 RESEARCH STRATEGY AND CONTENT

To perform the study in systematic and cover as much as details exist under several

constrains, the topic in each chapter was designed to study in different levels but

support to each other. Outline of research study is shown in Figure 1_7.

Chapter 2: This chapter is to illustrate experimental information, measuring

systems, and data interpretation methods, which they will be stated in details as

force transfer across shear crack and shear resisted by stirrup.

Figure.1_7: Research strategy.

Chapter 3: The experimental result corresponding with observation during

experimental work will be noticed. The results of load carrying capacity

compared with theoretically calculating equation are shown with some degree

of difference.

v

w,min

V

c

V

apply

V

s

V

y

- With

shear span to depth

ratio equal to 3.

- Vary stirrup ratio at 0.03%,

0.05%, 0.06% and 0.08%.

Experimental work

(Beam test under monotonic loading)

Chapter 2

Experimental Investigation

Specimen details.

Measuring systems.

Data interpretation methods

Chapter 3

Experimental Results

Beams results.

Strength comparisons.

Wcomd Analysis results.

Chapter 4

Mechanism in

Shear Resistance

Mechanism of stress

transfer

Assumption

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 8

Chapter 4: Leading to whole understanding in behavior of reinforced concrete

structure with a small amount of web reinforcement, this chapter is to

investigate and explain the mechanical of shear resistance by the means of

stress transferring across the crack and stress contributed by stirrups.

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 9

1.5 REFERENCES

1.) JSCE, “Report on The Hanshin-Awaji Earthquake Disasater: Investigation of

causes of damage to Civil Engineering Structures, Bridge Structures”, JSCE, V.1,

1996.

2.) Okamura, H., Saeki, M., and Kanatu, T., “History of Seismic Design Code for

Concrete Structure,” the scientific lecture for the great Hanshin-Awaji earthquake,

JSCE, Tokyo, 1996.

3.) Niwa, J., Yamada, K., Yokozawa, K., and Okamura, H., “Reevaluation of The

Equation for Shear Strength of Reinforced Concrete Beams without Web

Reinforcement,” Concrete Library International of JSCE, No.9, June 1987, pp.65-

84.

4.) Angelakos, D., Bentz, E. C., and Collins, M. P., “Effect of Concrete Strength and

Minimum Stirrups on Shear Strength of Large Members,” ACI Structural Journal,

V.98, No.3, May-June 2001, pp.290-300.

5.) Yoon, Y. S., Cook, W. D., and Mitchell D., “Minimum Shear Reinforcement in

Normal, Medium, and High-Strength concrete Beams,” ACI Structural Journal,

V.93, No.5, Sep.-Oct. 1996, pp.1-9.

6.) Frosch, R. J., “Behavior of Large-Scale Reinforced Concrete Beams with

Minimum Shear Reinforcement,” ACI Structural Journal, V.97, No.6, Nov.-Dec.

2000, pp.814-820.

7.) Collin, M. P., and Kuchma, D. K., “How safe are Our Large, Lightly Reinforced

Beams, Slabs, and Footings?,” ACI Structural Journal, V.96, No.4, July-Aug.

1999, pp. 482-490.

8.) Bazant, Z. P., and Sun, H. H., “Size effect in Diagonal Shear Failure: Influrence of

Aggregate Size and Stirrups,” ACI Material Journal, No.4, July-Aug. 1987,

pp.259-272.

9.) Vecchio, F. J., “Analysis of shear –Critical Reinforced Concrete Beams,” ACI

Structural Journal, V.97, No.1, Jan.-Feb. 2000, pp.102-110.

10.) Okamura, H., and Higai, T., “Proposed Design Equation for Shear Strength of

Reinforced concrete Beams without Web Reinforcement,” Concrete Library

International of JSCE, V.1, July 1993, pp.96-106.

11.) Park, R., and Paulay, T., “Reinforced Concrete Structures,” John Wiley &

Sons, New York, 1975.

12.) Russo, G., and Puleri, G., “Stirrup Effectiveness in Reinforced Concrete

Beams under Flexure and Shear,” ACI Structure Journal, V.94, No.3, May-June

1997, pp.227-238.

13.) Hassan, H. M., “ Shear Cracking Behavior and Shear Resisting Mechanism of

Reinforced concrete Beams with Web Reinforcement,” Doctoral Dissertation,

University of Tokyo, March 1988.

14.) JSCE, Standard Specification for Design and Construction of concrete

Structure, Part (Design), First edition, Tokyo, 1986.

15.) ACI committee 318, “Building code Requirements for Structural Concrete

and Commentary (ACI 318-83),” American Concrete Institute, Detroit, 1983,

pp.111.

16.) ACI committee 318, “Building code Requirements for Structural Concrete

and Commentary (ACI 318M-89/ACI 318R-89),” American Concrete Institute,

Detroit, 1989, pp.353.

17.) Canadian Standard Association, “Design of Concrete Structures for

Buildings,” CAN3-A23.3-M84, Rexdale, Ontario, 1984, pp.281.

General Introduction Chapter 1

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 10

18.) Canadian Standard Association, “Design of Concrete Structures,” CSA A23.3-

94, Rexdale, Ontario, 1994, pp.199.

19.) “AASHTO LRFD Bridge Design Specifications and commentary,” Second

Edition, (1998) and 2000 update, American Association of State Highway

Transportation Officials, Washington D.C., 1998, 2000.

20.) Krauthammer, T., “Minimum Shear Reinforcement Based on Interface Shear

Transfer,” ACI Structural Journal, V.89, No.1, Jan.-Feb. 1992, pp.99-105.

CHAPTER 2

EXPERIMENTAL DETAILS

Specimens Detail

Measuring System

Experiment Procedures

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 11

EXPERIMENTAL DETAILS

2.1 SPECIMENS DETAIL

2.1.1 Material Properties

For designing the reinforced concrete specimens and collecting the necessary data, the

material properties should be correctly known by conducting the material tests. Thus,

all principal materials used in constructing the reinforced concrete specimens, which

are steel bars and ordinary concrete, are tested and shown in following content.

Steel Reinforced Bars

The general properties of used steel bars, which all is deformed type but different in

grade between longitudinal and stirrup, are shown in Table.2_1. In the analysis, the

stress-strain curves of steel bars are necessary used as constitutive equation; therefore,

D4 stress-strain relation determined by regression method are shown in Figure.2_1.

The constitutive equation is easily to obtain by regression method since the D4 bar

shown non-exist of yield plateau. Therefore, it is proper to determine yield strength of

D4 bar by the 0.002 off set.

Stress-Strain Relation of D4 bars

0

100

200

300

400

500

0 0.01 0.02 0.03 0.04 0.05 0.06

Strain

Stress (Mpa)

part1 0 - 0.002

part2 0.002 - 0.003

part3 0.003 - 0.05

0.002 off set

Figure.2_1: Stress-strain curve and Constitutive equation of D4 bars.

Table.2_1: General properties of used deformed bars.

Steel Type

Nominal dia.

(mm.)

Yield Strength

(Mpa)

Ultimate Strength

(Mpa)

D4 (SD 295) 4.0 350 457

D10 (SD 345) 10.0 391 586

D22 (USD 685) 22.0 718 985

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 12

8 D22

D4 @ 80, 100, 130, 180

mm.

400 mm.

400 mm.

Clear cover

30

Clear cover 30

mm.

Ordinary Concrete

The casted concrete of specimens is ordinary concrete with the compressive strength

of 30 MPa at 28 days. Maximum aggregate size used as 20 mm. The curing method is

done by pouring water on the foam sheet that covered the specimens for first seven

days. Then, the beam specimens are cured by the air temperature in the laboratory.

2.1.2 Specimens Dimension and Parameters

According to the preliminary study in literature review, 4 reinforced concrete beams

are designed and used in experiment with the same dimension but varying amount of

web reinforcement to be less than 0.08%. As design is, the beams have unbalancing in

shear span ratio, a/d, which they approximately equal to 3 in left span and 1.5 in right

span. Respect to the target of the test, the right span has to highly reinforce with D10

bars to gain its ultimate strength higher than that of left span side. In Figure.2_2 a

and b, the beams cross-section and scale down specimens layout are shown,

respectively.

(a)

(b)

Figure.2_2: Tested beams layout.

Regarding to the beams layout and cross-section, the shear carrying capacity of each

beams were determined according to Niwa’s equation [1] parallel with superposition

method, (V

c

+V

s

), and they also used the material properties from material

experiments. The predicted shear strength of tested beams is shown in Table.2_2.

Ra = P/3

Rb = 2P/3

1080

mm

450 mm

540 mm 315mm

250 mm

2700

m

m.

300 mm

400 mm

D10@70

mm.

Vary number of stirrups

P

300 mm

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 13

Table.2_2: Shear carrying capacity of each tested beams.

Beam NO.

Spacing of web

Reinforcement (mm.)

V

s

(kN)

V

c

(Niwa)

(kN)

V

u

(kN)

1 D4 @ 80 40.58 160.81 226.6

2 D4 @ 100 32.47 163.35 187.8

3 D4 @ 130 24.97 161.06 190.8

4 D4 @ 180 18.04 166.6 187.5

2.2 MEASURING SYSTEMS

According to the research objectives, the mechanical of shear resistance have to be

correctly investigated and considered in tested beams. Thus, the careful measurement

methods have been designed according to the basis of shear resistance as the stress

transfer across the crack and the stress of web reinforcement. Measuring systems have

been desired on two microscopic models that can meaningfully explain local

behaviors in the specified parts. Finally, it is possibly that mechanical of shear

resistance in each two locations of beams can be accurately explained by these

measuring systems by employing two microscopic models.

2.2.1 Measurement of Stress Transfer across Crack Plane

a) Theoretical Background:

Buja Bujadham proposed the model to calculate the stress across cracks concrete, so

called Universal model for stress transfer across the crack [2,3], which it is actually

the generalization of Bi Li’s model, contact density model for stress transfer across

cracks concrete [4]. The stress transfer across cracks concrete can be imaged and

roughly illustrated in Figure.2_3. From figure, the opening and sliding of crack, and

, create the stress at contact unit of

s

, and summation of this stress at whole contact

unit results in the stress transfer across the crack

Figure.2_3: Stress transfer across the crack.

Contact density model concerns to the complex nature of crack surface, and then

represents it in mathematical ways by using two proposals and three basic

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 14

assumptions. Two basic proposals were crack geometry and contact stress direction

that shown in Eq.2-1 and 2-2, respectively.

Area of a contact unit :

dAdA

t

2-1

Contact stress direction :

s

2-2

Where, A

t

: whole surface area per unit crack plane

() : stochastic density function

s

: resultant contact angle

: contact angle before a unit deformed

Other three Eq.2-3, 2-4, and 2-5, were basic assumptions used in explain contact

density function, elasto-plastic model for contact stress, and effective ratio of contact

areas.

Contact density function:

cos21 2-3

Elasto plastic model:

'''

psc

R

2-4

Effective ratio of contact:

max

5.01exp1 GK 2-5

Where,

’

: local deformation in normal direction of crack unit

p

’

: local plasticity in normal direction of crack unit

Regarding to these equations, the stress crosses cracks are able to calculate in

somewhat specified loading paths, but not for complex loading paths same as mix-

mode loading path, crack opening and sliding, of shear crack in beams. The

unrealistic of contact stress direction proposal is the exclusion of frictional force,

which is produced at the contact unit since it undergoes in mix mode. Therefore,

application of normality rules is invalid to use in this research; comprising with the

actual, anisotropic behavior should be considered instead.

Beside that of concerning, the effect generated from mix-mode loading path, the

anisotropic plasiticity of mortar beneath aggregate, which generated from either the

nature of contact angle or the loading directions, and its fracture are accounted in

Universal model for stress transfer across cracks in concrete [3].

b) Measuring system

Contact extensometer and chips are designed to use in measuring the deformation of

shear crack opening and sliding of tested beams. By utilizing coordinate

transformations, the contact chips are located on the beam surface in both sides, north

and south surfaced, at the longer span part, which has a/d = 3.0. Contact chips are

cemented with the distance about 100 mm. apart from each others with the angle 0, 90,

135 degrees and 0,-45,-90 for north and south surfaces, respectively, as shown in

Figure.2_4.

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 15

(a) Chips coordinate (north surface of beams). (b) Chips coordinate (south surface of beams).

(c). Chips on the beam surface.

Figure.2_4: Measuring system of stress across the cracks

By the proposed method, after crack taken place, the angle of crack at the origin point

of contact chips coordinates are measured and utilized coordinate transformation

equation, Eq.2-6, which has been well known used in strain rosette.

3

2

1

333

222

111

2

2

2sin2cos12cos1

2sin2cos12cos1

2sin2cos12cos1

a

a

a

xy

y

x

2-6

Where,

i

: angle of i coordinate to tangential coordinate of crack

a

i

: deformation respect to i coordinate

x : crack deformation in parallel direction of crack plane

y : crack deformation in vertical direction of crack plane

xy : crack deformation in tangential direction of crack plane

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 16

c) Data Interpretation

From the measurement, deformation in 0, 90, 135 and 0, -45, -90 degrees related with

beam axis, and crack angle related to the beams axis are used in interpreting the crack

displacement in lateral and horizontal direction, y and xy to the crack plane,

respectively, as shown in the above equation.

Then, the universal model of stress transfer across the cracks is utilized to obtain the

amount of stress and force resisted by the aggregate interlocking mechanism. The

algorithm of model in calculating is shown in Figure.2_5. However, this outcome is

still in the crack plane coordination and it need to convert to the beam coordinate

again. By the coordinate transformation, the stress in Z direction, which is stress

contribution in shear resistance process of aggregate interlocking mechanism, can be

determined.

Figure.2_5: Algorithm of The Universal stress transfer across cracks concrete. [3]

2.2.2 Measurement of Strain of Web Reinforcement at Crack Plane

a) Theoretical Background: Bond-Slip-Strain Relationship of Steel bar

The tensile strain of reinforcement embedded in concrete has non-linear characteristic

depends on the embedment length. This is because the present of bond between the

reinforcing bar and surrounding concrete. With respect to the bond stress, the strain of

Input f

c

’

, G

max,

Initial

N = 150, d n

Given d

c

’

R

c

’

sin

.d

R

c

’

sin

s

.d

N = n

Next input

END

START

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 17

steel bar in several cases is shown in Figure.2_6 (a), (b), and (c), which are bond of

long embedment length, short embedment length, and bond of axial tension,

respectively.

(a) (b)

(c)

Figure.2_6: Strain of Embedded Reinforcing Bar. [5]

From the figures, the strain at specific point of reinforcing bar is nonlinearly reduced

respect to the distance from the crack section. Moreover, it is not necessary that the

same amount of slips have to be created by the same strain value, since the strain

distribution of embedded bar is affected by boundary conditions, which are the

embedment length, compressive strength of concrete, steel grade, and steel diameter.

Without considering the effect of strain value, many researchers failed to achieve

model to determine bond stress. On the other hand, Shima [6], proposed a universal

bond-slip-strain model for reinforced concrete, which take the effect of strain of

embedded bar at the considered point. Bond-slip-strain model is shown in Eq.2-7.

gss

o

, 2-7

Where, (,s) is local bond stress and

o

(s) is intrinsic bond stress when strain is zero

denoted by,

c

co

skfs 51ln

'

2-8

5

101

1

g 2-9

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 18

Where, f

c

’

: compressive strength of concrete

k : constant equal to 0.73

c : constant equal to 3,

s : non-dimensional slip equal to 1000S/d,

S : slip

d : diameter of steel bar

: strain of steel bar

Nevertheless, this experiment does not intend to measure the bond stress but it intends

to measure stress at the crack position. Fortunately, the strain at the crack position can

be determined by utilizing bond stress equation.

b) Measuring method

By utilizing a set of equations corresponding with strain from two nearing positions

along the embedded bar, stirrup, the strain at crack position can be indirectly

calculated. The set of equations according to the local bond behavior are shown in

Figure.2_8, which are bond-stress-slip equation, slip-strain relation, constitutive of

steel bar, and equilibrium equation, respectively.

According to this method, the strains at two points are located at 3 cm. apart from

each other. Furthermore, the position of strain gauges should be mouthed in the range

25 times of diameter from the crack section to ensure that the strain before yielding

can be investigated. With respect to this method, the approximate crack positions

should be determined in first place and it may be properly computed by some finite

element program, so called Wcomd (2 dimensions, plate element). Therefore, the

approximate solution by Wcomd is employed to locate the position of strain gauges at

each stirrup.

Figure.2_8: Equation for calculating strain of stirrup at crack plane.

Each reinforced concrete beam that analyzed by Wcomd shows almost the same crack

position in tested span as the sample in Figure.2_9; therefore, the crack formation can

aspect to be the same for simplicity in locating the strain gauge. The strain gauges

positions in each stirrup leg of all beam are shown in Table.2_3, which the height are

measured from the bottom of stirrup, the distances origin at the support, and the crack

heights are estimated from 45-degree crack tracing from the loading point.

Bond-slip-strain model:

gs

o

.

Slip-strain relation:

xS.

Constitutive of steel bar:

Equilibrium equation:

xdA

s

...

.A

s

(+).A

s

X

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 19

Figure.2_9: Crack pattern of tested beams.

Table.2_3: Stirrup strain position at each stirrup legs.

c) Data interpretation

From the measuring data, two strain values at two exact distances from the crack

section are input in the computer algorithm for iteratively determining the slip of the

farthest distance gauge. After the strain and slip of one exact location was exactly

known, the extrapolating of strain distribution can be done by assuming strain in next

position and then checking the equilibrium of stress between the bond and stress of

embed bar in each step. The algorithm of calculating the strain distribution, slip, and

stress at crack position is shown in Figure.2_10.

Specimen No.1 spacing 80 mm.Specimen No.2 spacing 100 mm.

Position (mm)

Height1

Height2

Height3

Position (mm)

Height1

Height2

Height3

1080 - - - 1080 - - -

1000 346 316 286 980 326 296 266

920 266 236 206 880 246 276 306

840 206 236 266 780 146 176 206

760 126 156 186 680 66 96 126

680 66 96 126 580 66 96 126

600 66 96 126 480 66 96

520 66 96 380 66 96

440 66 96 280 66 96

360 66 96 180 66 96

280

66

96

80

66

96

200 66 96

120 66 96

40

66

96

Specimen No.3 spacing 130 mm.Specimen No.4 spacing 180 mm.

Position (mm)

Height1

Height2

Height3

Position (mm)

Height1

Height2

Height3

1080 - - - 1080 - - -

950 296 266 236 900 266 296 326

820 186 216 246 720 86 116 146

690 66 96 126 540 66 96 126

560 66 96 126 360 66 96

430 66 96 26 180 66 96

300

66

96

26

0

170 66 96 26

40

66

96

26

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 20

Figure.2_10: Algorithm for calculating strain of web reinforcement at crack plane.

2.3 EXPERIMENT PROCEDURES

Specimens were set up in the loading frame with hand-pumping loading system. As

illustrated in Figure.2_11, the experiment set up before testing in each beam was

shown. The loading method was a load controlling and the measuring can be read at

the each loading steps equal to 30 kN. The load deflection can trace according to the

load-measured values and deflection measured value from the load cell and CDP,

respectively.

Figure.2_11: Specimen set up in the tested frame.

Assume

i+

i

+

i+1

)

S

i+1

= S

i

+ S

i+1

= f(S

i+1

).g(

i+1

)

Bond deterioration length

X

i+1

= X

i

+

i+1

< L

i+1

=

i

+

db.X /A

s

END

Input

f(S

1

).g(

f(S

1

+

D

S).g(

e

Assume S

1

Set B.C (S

1

,

at 1

st

point

db.X 0.01

Experimental Details Chapter 2

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement 21

2.4 REFERENCES

1.) Niwa, J., Yamada, K., Yokozawa, K., and Okamura, H., “Reevaluation of The

Equation for Shear Strength of Reinforced Concrete Beams without Web

Reinforcement,” Concrete Library International of JSCE, No.9, June 1987, pp.65-

84.

2.) Bujadham, B., Mishima, T., and Maekawa, K., “Qualitative Studies on

Mechanisms of Stress Transfer across Cracks in Concrete,” Procurement of JSCE,

V.17, No.451, Aug. 1992, pp. 265-275.

3.) Bujadham, B., and Maekawa, K., “ The Universal Model for Stress Transfer

across Cracks in Concrete,” Procurement of JSCE, V.17, No.451, Aug. 1992,

pp.277-287.

4.) Li, B., Maekawa, K., and Okamura, H., “ Contact Density Model for Stress

Trnasfer across Cracks in Concrete,” Journal of the Faculty of Engineering, The

University of Tokyo (B), Vol.XL, No.1, 1989, pp.9-52.

5.) Okamura, H., and Maekawa, K., “Nonlinear Analysis and constitutive Models of

Reinforced Concrete,” Gihodo-Shuppan, Tokyo, Japan, 1991.

6.) Shima, H., Chou, L. L., and Okamura, H., “ Micro and Macro Models for Bond in

Reinforced Concrete,” Journal of the Faculty of Engineering, The University of

Tokyo (B), Vol.XXXIX, No.2, 1987, pp.133-193.

CHAPTER 3

EXPERIMENTAL RESULTS AND INVESTIGATION

Strength and Determination Comparison

Discussion on Experimental Results

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

22

EXPERIMENTAL RESULTS AND INVESTIGATION

3.1 STRENGTH AND DETERMINATION COMPARISON

According to the aim of this research, the shear carrying capacity of reinforced

concrete member with a small amount of web reinforcement is the most important in

consideration and outcome. Thus, shear capacity of beams are now determined and

compared with the experimental result as it shown in Table.3_1.

Table.3_1: Comparison table.

Categories Beam 1 Beam 2 Beam 3 Beam 4

1.) Compressive strength (Mpa) 41.5 43.5 41.7 46.15

2.) Stirrup (%) 0.079% 0.063% 0.048% 0.035%

3.) V

s

(kN) 40.0 32.0 24.6 17.8

4.) Shear crack, V

cr

, (kN) 170.2 157.7 145.6 156.3

5.) Shear crack, V

c

, (kN) 160.81 163.35 161.06 166.6

6.) Shear capacity, V

u

, (kN) 226.6 187.8 190.8 187.5

7.) V

cr

/ V

c

1.06 0.97 0.9 0.94

8.) V

cr

+ V

s

210.2 189.7 170.2 174.1

9.) V

c

+ V

s

200.81 195.35 185.66 184.4

10.) V

u

/ V

cr

+V

s

1.08 0.99 1.12 1.08

11.) V

u

/ V

c

+V

s

1.12 0.96 1.03 1.02

12.) Failure mode S.C.

*

S.C. S.

**

S.C.

*

Shear compression failure

**

Shear failure

Refer to the table of comparison, the category number 11 and 12 show that the design

concept by superposition method, no matter what shear crack strength is taken from

either experiment or calculation, is good enough to predict the shear carrying capacity

of reinforced concrete members with a small amount of web reinforcement. Even

though the shear carrying capacity of each beam, except Beam 1, has mostly the same

level, this is going to quote and investigate into the mechanisms in next chapter.

3.2 DISCUSSION ON EXPERIMENTAL RESULTS

3.2.1 General Behaviors

Beam 1: The strongest beam

This beam contained the highest amount of web reinforcement, about 0.08%, which is

less than the design code mentioned in the first chapter. As observed during the test,

shear crack was taken placed at the shear load level equal to 170.2 kN. This beam did

not illustrate large and clear dropping of load deflection curve when the shear crack

was taken place. It can be seen from the load deflection curve, Figure.3_1 that the

shear crack load level did not affect in any drop of plotting.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

23

Load Deflection Curve of Beam 1

0

4

8

12

16

20

24

0 5 10 15

Deflection (mm)

Shear load (tf)

Figure.3_1: Load deflection curve of Beam 1.

After shear cracking formed, the load was increased further up to the failure point and

the beam was fail as shown in Figure.3_2. Regarding to failure load, the compression

zone was compression failure and followed by the large opening of shear crack since

the shear resisting in compression zone suddenly dropped and aggregate interlocking

at shear crack surface can not substitute shear resisting in compression zone. This

phenomenon simultaneously taken place with the cut-off of web reinforcement

illustrated in Figure.3_3.

Figure.3_2: Shear failure of Beam 1.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

24

Figure.3_3: Cut-off of Stirrup

Beam 2: A second highest amount of web reinforcement

Shear crack was taken place at load level in shear span equal to 157.7 kN, which is

slightly less than that of Beam 1. The crack formation of Beam 2 was generally

similar to Beam 1 without any special consideration. Shear crack formation, shear

failure, and load deflection curve are shown in Figure.3_4

Figure.3_4: Shear failure of Beam 2.

It is possible that the larger amount of web reinforcement ought to delay the time to

generate the perfect shear crack since the web reinforcement has highly possibility to

intersect with crack and effectively activate at the same load level as shown in

Figure.3_5 a and b. Similarly, it is too difficult to judge when the shear crack became

complete path since it does not occur suddenly as the case of beam without web

reinforcement. Therefore, it has possibility that the excess shear crack strength in last

beam compare to calculation is routed by them.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

25

(a) (b)

Figure.3_5: Possibility of crack intersect with stirrup

Load Deflection Curve of Beam 2

0

4

8

12

16

20

0 2 4 6 8 10

Deflection (mm)

Shear Load (tf)

Figure.3_6: Load Deflection Curve of Beam 2.

Onset of shear crack started, as it can be observed, Figure.3_6, load deflection curve

shows a little drop of graph after shear crack. It meant that the shear crack penetrated

to the compression quite fast, and then the load was able to increase further up to the

failure point. Similar to previous case, the compression zone firstly came up to the

compression failure, and then followed by the large shear crack opening and cut off of

web reinforcements in simultaneously.

Beam 3:

By the same manner with two previous beams but it is important to mention, shear

crack load of Beam 3 was observed at the shear load level equal to 145.6 kN that is

quite low when compares to previous cases. Even though this beam possessed the

same compressive strength and geometry as Beam 1, the shear crack loads of these

two beams were observed at different level of shear load. With respect to this

phenomenon, it is believed to be the same reason as explained in Beam 2 but it seems

to be clear since both beam had the same compressive strength. Shear crack formation,

shear failure, and load deflection curve are also shown in Figure.3_7.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

26

Load Deflection Curve of Beam 3

0

4

8

12

16

20

0 2 4 6 8

Deflection (mm)

Shear Load (tf)

Figure.3_7: Load Deflection Curve of Beam 3.

Figure.3_8: Shear Failure of Beam 3.

From the load deflection curve, the load had a little drop as shear crack taken place

and then the load was increased until the failure occurred. Different mode of failure

was observed in this beam since the compression zone did not fail, but the shear crack

was the controller instead.

Beam 4: Minimum web reinforcement

The smallest amount of web reinforcement beam, Beam 4, was created shear crack at

shear load level equal to 156.3 kN. Although the compressive strength of cylindrical

specimen was the highest in all beams, the shear crack load level was not the highest

among them. At the first place, this is believed that the initial state of crack did not

confine by the web reinforcement so that the stress at the crack front was propagate

very fast as aforementioned.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

27

Figure.3_9:Geometry of crack propagation.

In more details to support previously claimed, it was discovered that bond between

the concrete and the main reinforcement is a major cause for the initiation of inclined

shear cracking in RC beams [1]. Since this bond are shown to have excellent high

shear stress induce at the main reinforcement height. Its propagation believed to be

controlled by longitudinal cracking along the main bar, so-called horizontal crack [2],

which actually comes after inclined shear cracking. Therefore, the less amount of web

reinforcement usually yields lower load level to resist horizontal crack will show

larger and faster horizontal crack, which finally results in faster perfect shear cracking.

The illustrative sketching can be shown as Figure.3_9. However, this is not dowel

action developing by web reinforcement since the dowel action is believed and shown

to be affected by the position of first stirrup from the crack [3].

Load Deflection Curve of Beam 4

0

4

8

12

16

20

0 2 4 6 8 10

Deflection (mm)

Shear Load (tf)

Figure.3_10: Load Deflection Curve of Beam 4.

As shown in Figure.3_10 and 3_11, they illustrate about load deflection and shear

failure pattern. According to the load deflection curve, there is very large drop of it

since it was not enough amount of stirrup to confine the crack in both incline shear

crack and horizontal crack [3]. However, onset of shear cracking, the equilibrium

became satisfy again, and then the shear load can be increased further up to the failure

point. The failure mechanism and pattern in this beam is similar to Beam 1 and Beam

2, which the compression zone firstly crushed, and followed up by large crack

opening and cut-off of stirrups.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

28

Figure.3_11: Shear Failure of Beam 4.

3.2.2 Shear Carrying Comparison among Beams

Beams behaviors under experiment were explained as aforementioned; currently,

shear carrying capacity of all beam are going to be compared. Since the compressive

strength in each beam is different; therefore, the comparisons have to be done by

normalizing compressive strength. However, dividing the shear load by compressive

strength seems no meaning. Fortunately, there are some equations for determining

shear crack load and those equations used the compressive strength to be one of

parameter [4,5].

By normalizing the effect of compressive strength term, the remaining terms are

concerned with the beam geometries, and all beams had used the same geometry

during this experiment. Therefore, the comparing result by normalizing the

compressive strength term in shear crack prediction formula is used, and then it

consequently shows in Figure.3_12.

Load Deflection (Normailized fc' )

0

5

10

15

20

25

30

35

0 2 4 6 8 10

Deflection (mm)

ShearLoad

Normalized by fc'

Beam 1: Pw = 0.08%

Beam 2: Pw = 0.065%

Beam 3: Pw = 0.05%

Beam 4: Pw = 0.035%

Figure.3_12: Shear carrying capacity comparison by normalizing compressive strength.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

29

As observed from the graph, the effect of compressive strength on the shear crack

load was eliminated but the shear crack load and shear carrying capacity are still the

same, except Beam 1. It is meant that at a small amount of web reinforcement shear

carrying capacity cannot be exactly calculated by the concept of superposition;

however, the superposition method is still good enough to safely determine the shear

carrying capacity. As claimed, in actually, the bending members without web

reinforcement of the shear span ration, a/d, equal to 3.0 has some reserve strength

after the shear crack was taken place. It can be simply said that the shear strength of

the short span beam is not shear crack load.

3.2.3 Comparison between Several Calculation of Shear Strength

Several design codes, such as Eq.3-1, 3-2, 3-3, and 3-4, used superposition method by

selecting the concrete contribution term equal to the shear crack load. Currently, it

should be know that “Can these codes satisfy the shear failure beams with a small

amount of web reinforcement?” The calculation results are shown in Table.3_2.

ACI Committee 318-95 [6] V

cr

=

db

M

Vd

f

sc

.2.1716.0

'

3-1

CSA Simplification [7] V

cr

=

dbf

d

c

.

1000

220

'

3-2

CEB-FIP [8] V

cr

=

dbf

a

d

d

cs

s

..100

32.0

1.150

31

'

31

31

3-3

JSCE 1986 [9] V

cr

=

dbdpf

sc

.)100()100(9.0

4131

31

'

3-4

Table.3_2: Comparison between Experiment Results and Calculation of Several Codes.

Specimens.

No.

ACI

318-83

CSA

1994

CEB-FIP

Newzealand

NZS 3101

JSCE

1986

Beam 1 1.15 1.19 1.42 1.10 1.17

Beam 2 0.98 1.01 1.22 0.93 1.19

Beam 3 1.05 1.09 1.32 1.00 1.19

Beam 4 1.03 1.07 1.32 0.97 1.21

Note: The values in table obtained from dividing the experimental with calculation.

Mostly, the design code of each country used the shear crack load in estimating shear

carrying capacity in superposition method. Therefore, the superposition method is

seemingly applicable and good enough. With respect to safety, the comparisons table

shows that the testing values to calculating values ratio nearly to 1.0 and

underestimation in some codes, such as CEB-FIP and JSCE, since all of them were

provided some safety factor in the derivation processes. Especially, CEB-FIP shear

strength model was derived from fracture mechanic by assuming the dynamic mode

of splitting crack. This mode of splitting crack in the horizontal cracking is actually

not dynamic but the quasi-statistic by considering with the energy used in opening

conical crack at the bond face [10].

However, it has to be reminded again that the tested beam had quite short span ratio

but it is scale down in dimension from Shinkansen viaduct structures. As it is short,

the shear strength of the beam is not exactly the shear crack load but larger than that.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

30

Implying of inefficiency stirrup can be highly possible, and it can be said in advance

that simply said that the superposition method is not safe for long shear span ratio.

3.3 CONCLUSION

1.) The shear carrying capacity of reinforced concrete beam with a small amount of

web reinforcement can be safely determined by the superposition method, Vc+Vs.

Experimental Results and Investigation Chapter 3

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

31

3.4 REFERENCES

1.) Kim, W., and White, R.N., “Hypothesis for Localized Horizontal Shearing Failure

Mechanism of Slender RC Beams,” Journal of Structural Engineering, ASCE,

V.125, No.10, Oct. 1999, pp. 1126-1135.

2.) Kim, W., and White, R. N., “ Shear-Critical Cracking in Slender Reinforced

Concrete Beams,” ACI Structural Journal, V.96, No.5, Sep.-Oct. 1999, pp.757-

765.

3.) Poli, S. D., Prisco, M. D., and Gambarova, P. G., “Cover and Stirrup Effects on

The Shear Response of Dowel Bar Embedded in Concrete,” ACI Structural

Journal, V.90, No.4, July-Aug. 1993, pp.441-450.

4.) Niwa, J., Yamada, K., Yokozawa, K., and Okamura, H., “Reevaluation of The

Equation for Shear Strength of Reinforced Concrete Beams without Web

Reinforcement,” Concrete Library International of JSCE, No.9, June 1987, pp.65-

84.

5.) Okamura, H., and Higai, T., “Proposed Design Equation for Shear Strength of

Reinforced concrete Beams without Web Reinforcement,” Concrete Library

International of JSCE, V.1, July 1993, pp.96-106.

6.) ACI Committee 318, “Building Code Requirements for Reinforced concrete (ACI

318-95) and Commentary ACI 318-R95,” American Concrete Institute, Detroit,

1995.

7.) Canadian Standards Association, “Design of Concrete Structures for Buildings,”

CAN3-A23.3-M84, Rexdale, Ontario, 1984.

8.) Comite Euro-International Du Beton, “CEB-FIP Model Code 1990,” Thomas

Telford, London, 1993.

9.) JSCE, Standard Specification for Design and Construction of concrete Structure,

Part (Design), First edition, Tokyo, 1986.

10.) Gastebled, O. J., and May, L. M., “Fracture Mechanics Model Applied to

Shear Failure of Reinforced Concrete Beams without Stirrups,” ACI Structural

Journal, V.98, No.2, Mar.-Apr. 2001, pp.184-190.

CHAPTER 4

MECHANICAL IN SHEAR RESISTANCE

Mechanism of Stress Transfer

Mechanism of Web Reinforcement

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

32

MECHANICAL IN SHEAR RESISTANCE

In generally, the shear resistance can be divided into concrete part and web

reinforcement part. According to the contribution of concrete part, the aggregate

interlocking, dowel action, and shear in compression zone will be raised up after shear

cracking. However, in this research, the measured component was only the aggregate

interlocking or shear crack deformation since there is a limitation in techniques and

accuracy. Finally, it can be said that the shear resistance mechanism of reinforced

concrete beam with a small amount of web reinforcement was obtained.

4.1 MECHANISM OF STRESS TRANSFER

4.1.1 Crack Deformation

Due to the geometry of shear crack, some of contact chip groups are properly selected

to use in determining shear stress across the crack. Fortunately, all beams mostly

yielded the same crack pattern so that the shear stress across the crack can be directly

compared to each other. Before going to compare the shear stress cross the crack, the

location of measurement is shown by the circles in Figure 4_1.

Figure.4_1: Point of Measured Deformation.

At the considered location of crack deformation, the geometry of crack and beam

behavior have definitely correlation as Figure 4_2. Onset of shear crack, the crack

located in compression zone and the horizontal cracking, tension bars, mainly behave

in opening and rarely exist in sliding since the crack angle is almost parallel to the

beam axis. In other hand, as the horizontal crack opening, the inclined crack is going

under opening and sliding, simultaneously.

Figure.4_2: Crack Geometry and its deformation.

C

B

A

Compressive

zone

Inclined crack

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

33

The magnitude of crack opening and sliding can be considered by the length of the

arrow vector. By this figure, the above-mentioned are brightly understood the total

different at the compression zone and the inclined crack location.

Point A: Horizontal crack

Crack Opening

40

45

50

55

60

65

70

0 0.5 1 1.5

Crack width (mm)

Applied load (tf)

Pw 0.08% : N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.065% : S

Pw 0.05% : N

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Figure.4_3(a): Crack opening at the horizontal cracking.

In Figure.4_3 (a), beam specimen with web reinforcement ratio equal to 0.035%

shown the highest crack opening, whereas other beams with 0.065%, 0.05%, and

0.08% web reinforcement show smaller crack width at the same load level,

respectively. Even though the beam with web reinforcement ratio equals to 0.05%

should have crack width value larger than that of 0.065% but it is inversely perceived

from the measuring. However, beam with 0.05% web reinforcement ratio shown the

different in failure mode among others. Accordingly, it is believed that the reason

routed from different in failure mode. It can be concluded that the crack width of

beam at horizontal cracking will become larger respect to the smaller amount of web

reinforcement used.

Figure.4_3(b): Crack sliding at the horizontal cracking.

Definitely different from the crack opening at the horizontal cracking, the crack

sliding shown in Figure.4_3 (b) does not clearly show the good relation between crack

sliding with amount of stirrup used. However, it can be observed a little bit larger in

Crack Sliding

40

45

50

55

60

65

70

0 0.5 1 1.5

Crack slip (mm)

Applied load (tf)

Pw 0.08% :N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.065% : S

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

34

crack sliding in beam with 0.035% web reinforcement and almost same magnitude of

crack sliding in beam with 0.05%, 0.065%, and 0.08%, of web reinforcement.

Point B: Bottom of inclined crack

Crack Opening

40

45

50

55

60

65

70

0 0.5 1 1.5

Crack width (mm)

Applied Shear (tf)

Pw 0.08% : N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.065% : S

Pw 0.05% : N

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Figure.4_4(a): Crack opening at the bottom of shear cracking.

At the bottom of shear cracking, crack opening is largest when the web reinforcement

is smallest, and it became smaller when larger amount of web reinforcement is used

as observed in Figure.4_4(a). However, the beam with web reinforcement 0.05%

should have larger crack width than that of 0.065% but it is not actually since the

failure mode was different in beam that used 0.05%. These are also evidenced in

crack sliding as it shown in Figure.4_4(b).

Crack Sliding

40

45

50

55

60

65

70

0 0.5 1 1.5 2 2.5 3

Crack slip (mm)

Applied load (tf)

Pw 0.08% : N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.065% : S

Pw 0.05% : N

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Figure.4_4(b): Crack sliding at the bottom of shear cracking.

Furthermore, it can be observed that beam with web reinforcement 0.035% has very

large crack opening and sliding suddenly onset of shear crack initiated but it was not

the case for other beams.

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

35

Point C: Top of inclined crack

At the last location, tip of shear crack, the crack deformation, opening and sliding, is

shown in Figure.4_5 (a) and (b). With respect to the measuring result in figures, the

same behavior with last two locations can be observed.

Crack Opening

40

45

50

55

60

65

70

0 0.5 1 1.5

Crack width (mm)

Applied Load (tf)

Pw 0.08% : N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.065% : S

Pw 0.05% : N

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Figure.4_5(a): Crack opening at top of shear cracking.

More deeply in detail of crack deformation, it can be observed that the crack width

was almost the same in three reference locations but it was highest in crack sliding at

the bottom of shear crack width. Finally, again, it is absolutely possible to said that

when the larger amount of web reinforcement were used, the smaller crack

deformation in both opening and sliding without regarding to the location of total

shear cracking path.

Crack Sliding

40

45

50

55

60

65

70

0 0.5 1 1.5 2

Crack Slip (mm)

Applied Load (tf)

Pw 0.08% : N

Pw 0.08% : S

Pw 0.065% : N

Pw 0.05% : N

Pw 0.05% : S

Pw 0.035% : N

Pw 0.035% : S

Figure.4_5(b): Crack sliding at top of shear cracking.

4.1.2 Crack Deformation Path

From Fig.4_6, the plots of crack sliding to opening ratio at the lower side of inclined

crack are illustrated. In this figure, the applied shear load of all beams was normalized by the

maximum applied shear load of beam with highest shear carrying capacity, which was the

beam with web reinforcement ratio 0.08%. Except the beam with web reinforcement ratio

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

36

0.05% that failed in different manner compare with others, it can be observed that the plots of

crack sliding to opening ratios were approximately regarded to be the same level.

However, it can be also observed from this figure that the beams with smaller web

reinforcement had a large amount of crack sliding and crack opening just after the shear

cracking started. On the other hands, the beam with larger amount of web reinforcement

behaved only crack opening in the first state, and then gradually increased its sliding.

4.1.3 Shear Stress Cross Crack (Aggregate Interlocking)

By summing up all measured point, the aggregate interlocking contributed to resist

the shear load in each beam is calculated. With respect to results, the characteristic in

stress transfer across the crack of each beam can be easily seen from the graph as

shown in Figure.4_7. Start with Beam 2, 3, and 4, have similarly shear transfer, which

they are 100 kN up to 140 kN. Scattering is evidently observed but it is the limitation

of method used to measure the crack deformation. Then, last specimen, Beam 1, has a

great different stress transfer across the crack from others, where it starts with small

value after the crack has initially propagated until a little bit higher load than the

perfect shear crack taken place. After that, the shear stress across crack gradually rise

up to the 160 kN level, which was the highest among 4 specimens, and then the shear

failure is consequence.

Related to the beams behavior during the experiments, the three smallest in web

reinforcement specimens evidently show the dropping of load resistance since the

shear crack was suddenly opening and propagate as load deflection curves observed in

previous chapter. Thus, the suddenly jump to the maximum or near maximum of

stress transfer across the crack is the result of changing equilibrium, jump.

Nevertheless, it was not the matter for Beam 1 since the crack was not suddenly open

and propagate so fast that the load shown evidently dropping. Therefore, the shear

transfer did not rapidly increase but it delayed until the crack was widely open and

went under sliding. With respect to these considerations, the graph of stress transfer

across crack was shown in somewhat different patterns; however, the maximum shear

transfer can approximately the same with some degree of accuracy.

Crack deformation path

0.5

0.6

0.7

0.8

0.9

1

1.1

0 0.5 1 1.5 2

Sliding / Opening

Vapplied / Vmax

Pw = 0.035%

Pw = 0.05%

Pw = 0.065%

Pw = 0.08%

Fig. 4_6: Ratio of crack sliding to opening.

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

37

Shear Resisted by Aggregate Interlocking

0

20

40

60

80

100

120

140

160

180

140

150

160

170

180

190

200

210

220

230

Shear Load (kN)

Shear Resisted (kN)

Beam 1:Pw = 0.08%

Beam 2:Pw = 0.065%

Beam 3:Pw = 0.054%

Beam 4:Pw = 0.032%

Beam 2:Pw =0.065%

Beam 3:Pw = 0.054%

Beam 4:Pw = 0.032%

Beam 1:Pw =0.08%

Figure.4_7: Stress transfer cross crack.

Finally, the most important item is the crack opening and sliding. Due to these, in

reinforced concrete beam with a small amount of web reinforcement, it is possibly

that the beam with larger crack width corresponding to the larger sliding wins to the

same level of aggregate interlocking or stress across crack as beam with smaller crack

width and sliding since it can be previously observed in shear transfer of beam

number 2,3, and 4 that used 0.065%, 0.05%, and 0.035% of web reinforcement,

respectively. However, beam with web reinforcement 0.08% is approximately

respected to have same shear transfer of beams even the first state yielded the low

shear transfer and then became large shear transfer.

4.2 MECHANISM OF WEB REINFORCEMENT

4.2.1 Yielding of Web Reinforcement

After the data was collected and carefully considered, it can be said that the collected

data from the strain gauges mounted along the web reinforcement cannot be employed.

Thus, it seems that the yielding of web reinforcement cannot be known from the

direct measurement. However, it is known that crack width equal to the amount of

pull out of steel bar, which is 2 times of slip. By considering this relation, it should

suit to approximate the slip from the crack width as Eq.4-1.

2*Slip = Crack Width 4-1

Not only slip is calculated, but also strain at the crack should be found since the

objective is “Did the web reinforcement yield at the shear crack intersection?” With

respect to this reason, long embedment length terminology is considered to employ in

this case since the web reinforcement is a tiny size compared with the height of the

beams. Therefore, 2 more equations of strain-slip relation [1] for long embedded bar

are tool for the analysis in this state, and those equation are specified in following;

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

38

ss

s 35006 4-2

3

2

'

20

c

f

D

Slip

s 4-3

Where, s : normalized slip

s

: strain of web reinforcement

D : diameter of web reinforcement

f

c

’

: cylindrical compressive strength of concrete

At this state, after all related equations was introduced, the yielding strain from the

material test are going to be input in determining the normalized slip, and then slip

and crack width can be finally determined. Follow that describe, it can be finally

calculate that the crack width corresponding to the strain at yielding, which

determines by 0.002 offsets, is 0.42 mm, and then compare to the crack width of

every measured location along the shear crack, for example Figure.4_3, 4_4, and 4_5.

In conclusion, all web reinforcement intersected with the shear crack can be

considered as yielding state before shear failure of the beams according to the

previous figures of crack opening and sliding.

4.2.2 Other Mechanisms Contributed by Web Reinforcement

As frequently referred to the strain of web reinforcement, the effect of unachievable in

this value influences on the analysis of other mechanisms such as shear resistance in

compression zone and dowel action, which they cannot direct measure except adopt

from the indirect calculation. Therefore, it has to state in here that those mechanisms

[2] have not been investigated for reinforced concrete beam with a small amount of

web reinforcement currently.

4.3 CONCLUSION

1.) The beam with smaller amount of web reinforcement show larger in crack

opening and sliding. Except beam with 0.05% of web reinforcement, the crack

opening and sliding show some different from the claimed relation since the

failure is absolutely different.

2.) Beams with a small amount of web reinforcement have the same stress transfer

across the crack even the crack opening of them are totally different. Since the

larger of crack opening shows larger of crack sliding, the stresses in those beams

are finally maintained to be the same.

3.) All web reinforcement intersected by shear crack is considered to reach yielding

state by relying on the strain-slip model of long embedded steel bar and the

relation of crack width and slip.

Mechanical in Shear Resistance Chapter 4

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

39

4.4 REFERENCES

1.) Okamura, H., and Maekawa, K., “Nonlinear Analysis and Constitutive Models of

Reinforced Concrete,” Gihodo, Tokyo, 1991.

2.) Park, R., and Paulay, T., “Reinforced Concrete Structures,” John Wiley & Sons,

New York, 1975.

CHAPTER 5

CONCLUSION

Conclusion Chapter 5

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

40

CONCLUSION

Result of this research is very useful even the applicable length is very specific since the

experimental work was done only in the range of shear span equal to 3.0. However, it

can be said that most of viaducts and buildings are composed with the columns of shear

span ratio 3.0. According to the experimental results of four tested beams and their

corresponding measurement values of aggregate interlocking; therefore, it can be

confidently concluded as a unit as following:

1.) The shear carrying capacity of reinforced concrete beam with a small amount of web

reinforcement as shear span ratio 3.0 can be safely determined by the superposition

method, V

cr

+V

s

.

2.) The beams with smaller amount of web reinforcement showed larger in crack opening

and sliding. Except beam with 0.05% of web reinforcement, the crack opening and

sliding showed some different from the claimed relation since the failure is absolutely

different.

3.) All beams have the same stress transfer across the crack even the crack opening and

sliding of them were totally different. Since the larger of crack opening showed the

larger of crack sliding; therefore, the stresses in those beams are finally maintained to

be the same.

CHAPTER 6

RECOMMENDATIONS OF FURTHER STUDY

Recommendations of Further Study Chapter 6

Shear Behavior of Reinforced Concrete Beams with A Small Amount of Web Reinforcement

41

RECOMMENDATIONS OF FURTHER STUDY

Based on the experimental results according to the experimental plan and problems in

analyzing procedures, it is better to specify some recommendations for further study as

following:

1.) Improving on measuring systems or data collecting method, for example stress

transfer across crack and strain of web reinforcement at the crack position, in

order to improve the accuracy and more detail understanding in the depth of

behavior.

2.) Extending the measuring systems or data collecting method to other locations or

items, for example the shear resistance of compression zone and that of dowel

action.

3.) More widely parametric studies are necessary to continue since this behavior

seemingly to different in longer shear span ratio, compressive strength, and

absolutely different in reversed cyclic loading.

APPENDIX A

Crack Mapping

BEAM WITH WEB REINFORCEMENT 0.08%

North side

South side

## Comments 0

Log in to post a comment